Physical-Chemical and Mechanical Characterization of the Bast Fibers of Triumfetta cordifolia A.Rich . from the Equatorial Region of Cameroon

The project consists in the implementation of a biocomposite based on tannin resin and natural rubber matrices with the bast fibres of Triumfetta cordifolia A.Rich. “Okong” from the equatorial region of Cameroon as reinforcement. A study of this still little known fibre is necessary. This paper eva-luates the physico-chemical and mechanical characteristics of the fibers. The fibers are extracted by us. A series of experiments is conducted for this pur-pose: morphological observation with a scanning electron microscope (SEM); density evaluation with a helium pycnometer; absorption rate evaluation according to the protocol available in the literature, Fourier Transform Infrared Spectrometry (FT-IR), chemical composition evaluation according to ASTM 1972 and ASTM 1977 standards, thermogravimetric analysis (TGA) and tensile tests on fiber bundles according to NF T25-501-3. The results show that the fiber is made up of several elementary fibers with oval cross-sections. A density of 1.477 g/cm 3 close to that of hemp. These fibers have a water absorption rate of 342.5%, which correlates with the presence of free hydroxyl functional groups obtained from the spectrometry study (FT-IR). Chemical analysis reveals that the fiber is made up of celluloses (44.4%), hemicelluloses (30.8%), lignins (18.9%), pectins (3.3%), waxes (0.5%) and minerals (2.1%). In addition, we learn that the fibers studied dehydrate at 11.49%, showing a notable thermal stability around 235˚C with a peak thermal decomposition of cellulose located at 420˚C. In terms of mechanical behaviour, the results reveal that the fibers offer a Young’s modulus in traction of 12.4 ± 6.9 GPa, a tensile strength of 526 ± 128 MPa and an elongation at break of 2.25%. The information thus obtained makes it possible to place these fibers in the same fiber group as flax and jute. They could therefore be used for the same types of applications. They also inform us that these fibers can withstand the temperatures of composite shaping by thermocompression.


Introduction
The selective choice of a reinforcing fiber is of the utmost importance and requires knowledge of all the physico-chemical, mechanical and thermal properties in order to produce good quality composite materials. To this end, natural fibers are governed by a set of parameters, including: chemical composition, crystallinity index (CrI) of the cellulose, microfibrillar angle (MFA), good length/diameter (L/D) ratio of the fiber, good tensile strength, good elongation capacity and low sensitivity to temperature and humidity variations [1].
In order to develop natural composites based on plant resins, reinforced with bast fibers of Triumfetta cordifolia A.Rich. (TC) harvested in Cameroon, knowledge of these parameters is essential for the overall performance of the composite.
To date, Senwitz et al. [2], have carried out a characterisation study of TC fibers and the results reveal that the property values obtained from TC fibers harvested in the northern zone of Angola are comparable to those of commercial jute, flax, hemp and kenaf fibers. They also reveal the potential required as a reinforcement for composites. Indeed, these results show an average Young's modulus of (12.5 -53.4 GPa), tensile strength of TC fibers (209.  and (1.56% -1.56%) deformation at break. They also have a density of (1.16 -1.41 g/cm 3 ), a microfibril angle of (7˚ ± 5˚), and finally a chemical composition consisting of Holocellulose (72.26% -87.90%), lignin (9.90% -13.67%), and extract content (0.70% -3.10%).
In view of these encouraging properties, develop biocomposites based on plant resins with TC bast fiber reinforcements. In the hypothesis of the use of this fiber, in the reinforcement of plant matrices such as tannin extracted from Aningré or Abam (Aningeria superba) and natural rubber latex (NR) derived from Brazilian rubber grown in Cameroon, shaping requires knowledge of the degradation temperatures of the fibers [3] [4]. It is therefore imperative that the degradation profile and in particular the thermal stability of the fibers be known before their use in composite applications [5]. For the moment, this information  [8]. Also, most of the specimens with vegetable fiber reinforced vulcanized natural rubber and tannin matrices are usually processed by thermocompression [9]. It is therefore imperative to complete the knowledge of the fiber.
After all, the characteristics of plant fibers vary from one geographical area to another, so it is advisable to repeat the determination of the characteristics of the fiber already available in the literature.
In this article, we present the fiber extraction procedure. Microscopic examination was performed using a Hitachi 3000 scanning electron microscope (SEM). The pycnometer was used to evaluate the density of the fibers. Chemical analysis was performed to determine the content of cellulose, hemicellulose in lignin, pectins in waxes and minerals. Moisture content was calculated. By means of infrared spectroscopy (FT-IR) the structural functional groups were identified. The thermal behaviour of the fiber was evaluated by thermogravimetric analysis (TGA). Finally, the tensile properties of fiber bundles were measured using a FAVIMAT+ machine.

Extraction of Triumfetta cordifolia Fibers
The raw material Figure 1

Scanning Electron Microscopy Analysis
The microscopic examination and the calculation of the effective cross-section are performed using Hitachi 3000 Scanning Electron Microscopy (SEM). In agreement A batch of staple fibers was mechanically opened on the Laroche opener at 1200 rpm. A type of process used in pre-treatment for composite/non-woven reinforcement type applications. The fibers are separated manually, aligned to have a homogeneous parallelization of the fibers and then introduced into the sample holder of the scanning electron microscope after metallization. All images were taken at an accelerating voltage of 15 kV. Image Pro Premier  software is then used to determine the fiber dimensions.

Density Measurements
The fibers were previously dried in the oven at 60˚C for 24 hours and cooled in a desiccator at room temperature. The density of each sample is determined by measuring the dry fiber weight determined with a 0.0001 g precision balance and then introduced into the container of the Quantchrome Helium Pycnometer MVP-6DC Pycnometer Instruments. The operating principle of the helium pycnometer is based on the gas law [11], defined by Equation (1). The volume of the fiber is determined by measuring the pressure variation experienced by the fluid due to the displacement of the fluid in constant volume by the test sample.
This method is in accordance with [12].
where ρ is the density (g/cm 3 ), V f is the fiber weight (g), V p is the sample volume (cm 3 ), V c is the sample orifice volume (cm 3 ), V r is the reference volume (cm 3 ), P 1 is the pressure measured after pressurizing the reference volume (V r ) (PSI), P 2 is the pressure measured after including the cell volume (V c ) (PSI).

Water Absorption
The TC fiber water absorption test was performed according to the method of [13]. Seven samples were prepared and the mean percent water absorption was calculated using Equation (2). The samples were first weighed as M 0 and then immersed in fresh water for 24 hours at room temperature. After 24 hours of immersion, the samples were reweighed as M 1 .

A Fourier Transform Infrared (FTIR) analysis is performed using a Shimadzu
IRAffinity-1 CE Shimadzu instrument equipped with a diamond crystal operating in ATR mode. The infrared spectrum is recorded from 500 to 4000 cm −1 by accumulation of 32 scans with a resolution of 4 cm −1 .

Chemical Characterization
The determination of the content of cellulose, hemicelluloses, lignin, pectin and waxes is carried out in accordance with ASTM 1972 and ASTM 1977. The method used is a method by successive extraction of the components of the fibrous material by solvents from a mass of approximately 2 g of ground and dried fiber.
The first extraction the alcohol-toluene mixture which will dissolve the waxes and fats and then a second extraction is carried out with hot water at 90˚C which will allow the determination of the quantity of mineral salts as well as the low

Thermogravimetric Analysis (TGA)
The thermogravimetric analysis is performed on an analyzer (TGA) using the NETZSCH STA 449F3 Jupiter (Germany) under constant air from 25˚C to 700˚C at a heating rate of 10˚C/min. About 10 mg of the sample was used.

Tensile Strength
The test specimens were first separated manually and stored in a conditioning chamber at a controlled temperature of 20˚C ± 1.5˚C and a relative humidity of 60% ± 1% for 24 hours. Tensile tests on fiber bundles were carried out on a FAVIMAT+ machine. For this purpose, 44 fibers were tested at a speed of 5mn/min in accordance with the NF T25-501-3 standard. The tests were carried out using a 3200 cN force sensor, the holding length was 10 mm. The effective cross-section was calculated from a scanning electron microscopy (SEM), using a Hitachi 3000 instrument, in accordance with [14].

Scanning Electron Microscopy Analysis
Like flax and hemp, TC fibers are located at the periphery of the stem.    shows the cross-section of the lumen structure. This lumen is oval in shape, this shape and large aperture could be due to the efforts applied during the preparation of the fibers. Indeed, the fibers were separated (opened) with the Laroche opener. Figure 2(b) is a longitudinal view of the TC fiber. It shows that there are impurities on the surface, and this structure has many burrs, which is due to the absence of surface treatments. However, the strength of the bundle structure is much lower than that of the elementary cell (see Table 4).

Density
The density of TC fiber is low at 1.477 ± 0.016 g/cm 3 , but close to (1.41 g/cm 3 ) compared to the same species [2]. Moreover, it should be noted that it is similar to that of flax fibers and (1.50 g/cm 3 ) of hemp fibers (1.47 g/cm 3 ) respectively [16] [17] and therefore TC fiber can be used in the same applications as the latter.

Water Absorption
Water absorption by TC fibers is high at 342.3%. This highly hydrophilic character is also attributed to the presence of hemicelluloses [18], but also to the high group content of free hydroxyl groups [13], responsible for moisture sorption (see IR-spectrum in Figure 3) and affects the physical and mechanical properties of our fibers [18]. Also the high porosity observed on the microstructure ( Figure 1). According to [19], this character leads to drops in stiffness and the appearance of cracks within the composite. Nevertheless, it should be noted that this disadvantage could still be improved by a surface treatment.

FTIR-ATR Spectrometry
The spectral analysis of the TC fibers obtained gives us the FTIR-ATR spectrum ( Figure 3).
The infrared spectrum obtained above shows the positions of the well-defined bonds of the inter and intramolecular network of cellulose, as well as the free hydroxyl groups of hemicellulose [20]. Moreover, Célino et al. [16] have observed   1234 Acetyl groups (hemicellulose) [16] 1031 C-O stretching ring (cellulose and hemicellulose) [16] 662 C-OH out of plane bending (cellulose) [20] [25] that this absorption band is characteristic of the presence of liquid water more or less bound to the polymeric network that constitutes the natural fibers. The second peak located at 2917 cm −1 represents the (-CH) group present in hemicellulose and cellulose [16] [21] [22] [23]. However, we observe an evidence by the decrease of the signal of the characteristic peak at 1728 cm −1 which corresponds to symmetrical elongation of ester group (C=O of carboxylic acids) present in pectins, waxes and acetyl groups present in hemicelluloses [7] [23]. Also the absorption of this peak confirms the hydrophilic nature of the natural fiber [21]. The region of the spectrum in the band between 1506 cm −1 and 1605 cm −1 is characteristic of the symmetrical aromatic (C=C) elongation present in lignin. The observable peak around 1315 cm −1 is characteristic of the vibration of the -CH bond and the aromatic -CO group present in polysaccharides. From there, at 1031 cm −1 , peaks corresponding to stretching bonds of the C-O ring are found. These bonds are characteristic of cellulose and hemicellulose [16]. Finally, the characteristic peak at 662 cm −1 is attributed to cellulose [20] [25]. These results show that TC fiber is composed of cellulose, hemicellulose, lignin, pectins, waxes and polysaccharides. It is therefore similar to known plant fibers such as jute, sisal, flax and hemp [22] [26].

Chemical Composition
The chemical composition of the TC fiber and the values of other vegetable fibers are given in Table 2. In contrast to the work of Senwitz et al. [2], which gives the holocellulose (72.26% -87.90%) and extract content (0.70% -3.10%) contents, this chemical analysis goes as far as to dissociate the cellulose, hemicellulose, pectins, waxes and minerals in terms of content. It appears that TC fiber contains 44.4% cellulose, thus less than hemp or flax but close to kenaf, jute and coconut fiber in the literature [27] [28] [29]. This content also indicates that its fibers could find very good applications in composites and textiles. On the other hand, the 30.8% hemicellulose content is higher compared to conventional fibers [27] [28] [29] [30]. This is due to its highly hydrophilic nature, which is responsible for the absorption of water due to the presence of free hydroxyl groups in its structure [18] [19] [20]. The percentage of lignin (18.9%) is similar to that of flax and kenaf [27] but it is high compared to the work of Senwitz et al., [2]. These studies also note that the high lignin and hemicellulose content increases with retting time. Consequently, the considerable amount of pectins (3.3%) and hemicellulose that is not removed during retting results in a significant reduction in the stiffness and strength of TC fibers [2]. Finally, TC fibers have (2.1%) minerals and also a very low wax content (0.5%).

Thermogravimetric Analysis (TGA)
The results of the thermogravimetric analysis (TGA) of the fiber under study give us the TG-DTG curves in Figure 4. A. E. Mewoli et al. These curves are similar to those obtained for linen, jute, banana and hemp [7] [13] [32] [33]. They show three main regions of mass loss: An initial mass loss, observed in the temperature range 75˚C -144˚C, of about 11.49%, which is mainly attributed to fiber dehydration [17]. This mass loss stabilizes at 235˚C and is the locus of thermal stability of the fiber [33]. A further loss of mass will occur above 235˚C (46.02%), due to the decomposition of the less thermally stable elements such as non-structural hemicelluloses [21] [32] [34], fats and waxes [35]. The inflection point observed at about 336˚C, (loss of mass of about 43%), would correspond to the destruction of part of the constituents (cellulose in particular and the oxidative degradation of carbonized residues) [33]. The DTG curve of the TC fiber shows a peak at 420˚C (mass loss of 72%) which is due to the thermal decomposition of the cellulose [7] [33]. According to [21] [22], lignin is more heat resistant and decomposes last. This decomposition is observed in the 420˚C -482˚C region. Above 482˚C, mass loss becomes very slow and a stable residue is formed. A residue of 12.69% of the TC fiber remains after heating to 700˚C. Table 3 compares the degradation characteristics of the fiber under study with those of other known plant fibers.
It can be observed that TC has an important residue compared to other vegetable fibers except banana fibers, which would confirm a better temperature resistance.

Tensile Strength of TC fiber
The tensile tests reported in Figure 5(a) show that the TC fiber is a fiber with low elasticity and its mode of rupture qualifies it as brittle. Table 4 through the associated values show that these fibers have low mechanical properties compared to those of the same plant from the work of Senwitz et al. [2] except for elongation they are the most extensible.   tions (2.25%) are similar to those of jute or sisal in the literature [30] [31], but also to that of untreated TC (2.55%) from the work of Senwitz et al., [2]. The Young's modulus of the fiber samples from TC (12.4 GPa) is rather low compared to that of TC (53.4 -59.8 GPa) routed between three and six weeks respectively [2]. Similar values show a stiffness comparable to that of cotton (5.50 -12.6 GPa) or jute (10 -26.5 GPa) [31], (6.3 -26 GPa) [22] and RC (2.3 -17 GPa) [38]. All these mechanical properties (σ, E, ε) of TC fibers are still superior to those of NA fiber [39]. These fiber tensile results also support the 44.4% cellulose content obtained in the chemical composition. Also, many factors such as extraction methods, fiber morphology, climate, age (or maturity stage), different geographical area could influence these mechanical properties [31].

Figures 5(b)-(d) and
In the end, TC fibers are flexible compared to hemp and flax fibers as these have a low Young's modulus. The softer a fiber is, the lower its Young's modulus and therefore it finds applications in composites and textiles [1].

Conclusion
The bast fibers of Triumfetta cordifolia A.Rich., extracted by retting, have been characterized. The results reveal that the fiber consists of several elementary fibers with oval cross-sections. They have a density of 1.477 g/cm 3 . Although the water absorption of these fibers is quite high, it can be improved by surface treatment of the fiber. The fiber consists of cellulose, hemicellulose, lignin, pectins and minerals. Its 44.4% cellulose content in particular gives it tensile properties similar to those of jute, flax and kenaf. This makes them suitable for the same applications. Moreover, in terms of mechanical properties, TC fiber has a relatively low tensile stress and high elongation at break compared to the same species in the literature. This difference could be justified by the different geographical location of fiber harvesting. This study also shows that the fiber can withstand the processing temperatures of the proposed composites without degradation. It is therefore suitable for the implementation of composites by thermocompression. This work has therefore confirmed that TC fibers are suitable for the reinforcement of composite materials. In perspective, this work will be complemented by surface treatments of TC fibers and then biocomposites will be manufactured with matrices of tannin resins and natural rubber latex reinforced with treated and untreated TC fibers.